A stable and highly selective metalloporphyrin based framework for the catalytic oxidation of cyclohexene.
Xia, Zhinan; Li, Fengyan; Xu, Lin; Feng, Pingyun; Dalton transactions (Cambridge, England : 2003) 49 (2020) 11157–11162; doi:10.1039/d0dt01420f

data_7704857
_publ_section_title
;
 A stable and highly selective metalloporphyrin based framework for the
 catalytic oxidation of cyclohexene.
;
_journal_issue                   32
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              11157
_journal_page_last               11162
_journal_paper_doi               10.1039/d0dt01420f
_journal_volume                  49
_journal_year                    2020
_chemical_formula_sum            'C50 H43 Mo2 N5 O16'
_chemical_formula_weight         1325.77
_space_group_crystal_system      orthorhombic
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2020-07-09 deposited with the CCDC.	2020-07-17 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   24.2727(9)
_cell_length_b                   35.9510(13)
_cell_length_c                   7.6427(3)
_cell_measurement_reflns_used    9864
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.124
_cell_measurement_theta_min      2.583
_cell_volume                     6669.2(4)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SMART'
_computing_molecular_graphics    'DIAMOND (Brandenburg, 1999)'
_computing_publication_material  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_computing_structure_solution    'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.434
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device_type  'Bruker SMART APEX CCD'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0747
_diffrn_reflns_av_unetI/netI     0.0449
_diffrn_reflns_Laue_measured_fraction_full 0.434
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       6
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            18695
_diffrn_reflns_point_group_measured_fraction_full 0.434
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         18.838
_diffrn_reflns_theta_min         1.771
_diffrn_source                   'fine-focus sealed tube'
_exptl_absorpt_coefficient_mu    0.433
_exptl_absorpt_correction_T_max  0.996
_exptl_absorpt_correction_T_min  0.990
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
'SADABS 2014/5 (Bruker, 2014) was used for absorption correction. 
R(int) was 0.0870 before and 0.0747 after correction. 
The Ratio of minimum to maximum transmission is 0.9939. 
The \l/2 correction factor is not present.' 
;
_exptl_crystal_colour            dark-red
_exptl_crystal_density_diffrn    1.320
_exptl_crystal_description       block
_exptl_crystal_F_000             2360
_exptl_crystal_size_max          0.030
_exptl_crystal_size_mid          0.020
_exptl_crystal_size_min          0.010
_platon_squeeze_details
;
TITL test1 in Pnma
CELL   24.2727   35.9510    7.6427     90.00     90.00     90.00
SPGR Pnma
Q101 0.434 0.243 0.252 !       2.55 eA-3
C102 0.291 0.947 0.082 !       2.31 eA-3
Q103 0.930 0.203 0.232 !       2.31 eA-3
C104 0.294 0.936 0.139 !       2.25 eA-3
C105 0.842 0.921 0.517 !       2.02 eA-3
Q106 0.500 0.500 0.000 !       1.89 eA-3
C107 0.780 0.573 0.248 !       1.67 eA-3
C108 0.681 0.449 0.967 !       1.66 eA-3
Q109 0.005 0.248 0.375 !       1.60 eA-3
C110 0.282 0.984 0.066 !       1.56 eA-3
C111 0.249 0.461 0.686 !       1.42 eA-3
Q112 0.993 0.710 0.205 !       1.29 eA-3
Q113 0.954 0.736 0.058 !       1.27 eA-3
C114 0.176 0.485 0.409 !       1.22 eA-3
C115 0.765 0.458 0.656 !       1.19 eA-3
Q116 0.042 0.747 0.875 !       1.14 eA-3
Q117 0.469 0.253 0.719 !       1.14 eA-3
C118 0.486 0.211 0.166 !       1.14 eA-3
C119 0.641 0.461 0.073 !       1.09 eA-3
Q120 0.437 0.753 0.625 !       1.08 eA-3
C121 0.685 0.451 0.237 !       1.05 eA-3
Q122 0.006 0.768 0.986 !       1.01 eA-3
C123 0.803 0.475 0.702 !       0.98 eA-3
Q124 0.533 0.778 0.687 !       0.95 eA-3
Q125 0.275 0.928 0.969 !       0.95 eA-3
Q126 0.491 0.206 0.439 !       0.94 eA-3
C127 0.246 0.506 0.254 !       0.94 eA-3
Q128 0.813 0.583 0.617 !       0.93 eA-3
Q129 0.562 0.484 0.153 !       0.92 eA-3
Q130 0.391 0.964 0.053 !       0.88 eA-3
C131 0.736 0.995 0.108 !       0.87 eA-3
Q132 0.837 0.751 0.437 !       0.85 eA-3
Q133 0.040 0.732 0.438 !       0.84 eA-3
C134 0.764 0.055 0.947 !       0.82 eA-3
Q135 0.180 0.010 0.065 !       0.80 eA-3
C136 0.005 0.290 0.207 !       0.80 eA-3
C137 0.995 0.710 0.793 !       0.80 eA-3
Q138 0.326 0.601 0.380 !       0.79 eA-3
Q139 0.503 0.250 0.406 !       0.77 eA-3
Q140 0.969 0.305 0.560 !       0.76 eA-3
C141 0.813 0.991 0.738 !       0.76 eA-3
Q142 0.927 0.164 0.241 !       0.76 eA-3
C143 0.235 0.014 0.081 !       0.75 eA-3
Q144 0.438 0.269 0.728 !       0.74 eA-3
Q145 0.938 0.231 0.772 !       0.74 eA-3
Q146 0.319 0.034 0.005 !       0.74 eA-3
Q147 0.319 0.749 0.469 !       0.73 eA-3
Q148 0.078 0.725 0.303 !       0.73 eA-3
Q149 0.765 0.912 0.862 !       0.73 eA-3
Q150 0.703 0.419 0.215 !       0.70 eA-3
Q151 0.422 0.251 0.125 !       0.69 eA-3
Q152 0.795 0.496 0.278 !       0.68 eA-3
Q153 0.930 0.217 0.055 !       0.67 eA-3
Q154 0.196 0.713 0.483 !       0.67 eA-3
Q155 0.343 0.972 0.251 !       0.66 eA-3
C156 0.781 0.523 0.831 !       0.66 eA-3
Q157 0.600 0.426 0.112 !       0.65 eA-3
Q158 0.227 0.749 0.406 !       0.65 eA-3
Q159 0.148 0.969 0.373 !       0.65 eA-3
C160 0.781 0.554 0.892 !       0.65 eA-3
Q161 0.372 0.164 0.287 !       0.64 eA-3
Q162 0.500 0.782 0.165 !       0.63 eA-3
Q163 0.607 0.517 0.213 !       0.63 eA-3
Q164 0.194 0.936 0.151 !       0.63 eA-3
Q165 0.994 0.305 0.709 !       0.63 eA-3
Q166 0.590 0.728 0.039 !       0.63 eA-3
C167 0.984 0.781 0.860 !       0.62 eA-3
Q168 0.907 0.236 0.484 !       0.61 eA-3
Q169 0.860 0.495 0.535 !       0.61 eA-3
Q170 0.088 0.801 0.467 !       0.61 eA-3
C171 0.453 0.211 0.062 !       0.61 eA-3
Q172 0.054 0.805 0.340 !       0.60 eA-3
Q173 0.554 0.780 0.450 !       0.60 eA-3
Q174 0.889 0.253 0.000 !       0.60 eA-3
Q175 0.844 0.811 0.584 !       0.60 eA-3
C176 0.446 0.321 0.577 !       0.60 eA-3
Q177 0.827 0.571 0.148 !       0.59 eA-3
Q178 0.539 0.695 0.319 !       0.59 eA-3
Q179 0.017 0.229 0.561 !       0.59 eA-3
C180 0.816 0.589 0.898 !       0.59 eA-3
Q181 0.205 0.649 0.429 !       0.59 eA-3
C182 0.740 0.361 0.608 !       0.58 eA-3
Q183 0.351 0.017 0.932 !       0.58 eA-3
C184 0.849 0.892 0.407 !       0.58 eA-3
Q185 0.572 0.080-0.017 !       0.57 eA-3
Q186 0.063 0.433 0.463 !       0.57 eA-3
Q187 0.625 0.052 0.256 !       0.55 eA-3
Q188 0.036 0.287 0.331 !       0.55 eA-3
Q189 0.784 0.791 0.473 !       0.54 eA-3
C190 0.959 0.183 0.250 !       0.54 eA-3
Q191 0.124 0.750 0.250 !       0.53 eA-3
Q192 0.982 0.329 0.348 !       0.52 eA-3
Q193 0.444 0.961 0.047 !       0.52 eA-3
Q194 0.366 0.572 0.309 !       0.51 eA-3
Q195 0.204 0.893 0.385 !       0.51 eA-3
Q196 0.345 0.829 0.055 !       0.51 eA-3
Q197 0.947 0.795 0.033 !       0.50 eA-3
;
_refine_diff_density_max         1.656
_refine_diff_density_min         -0.818
_refine_diff_density_rms         0.122
_refine_ls_extinction_coef       0.0008(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.014
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     321
_refine_ls_number_reflns         2664
_refine_ls_number_restraints     30
_refine_ls_restrained_S_all      1.012
_refine_ls_R_factor_all          0.0867
_refine_ls_R_factor_gt           0.0778
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0828P)^2^+140.7050P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1952
_refine_ls_wR_factor_ref         0.2016
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2320
_reflns_number_total             2664
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0dt01420f2.cif
_cod_data_source_block           mo1_sq
_cod_depositor_comments          'Adding full bibliography for 7704857.cif.'
_cod_database_code               7704857
_shelx_estimated_absorpt_t_min   0.987
_shelx_estimated_absorpt_t_max   0.996
_shelxl_version_number           2014-3
_shelx_res_checksum              98834
_platon_squeeze_void_probe_radius 1.20
_shelx_fab_checksum              1110